and Strength of Timbers. 
129 
I Number of experi- 1 
ment. 
Names of the 
woods. 
Specific gravity. 
Greatest weigh! 
and deflection 
while the elas- 
city retnainet 
perfect. 
Breaking weigt in lbs. 
Ultimate deflection in 
inches. 
Value ol 
U 
from the 
formula 
/ a 
~ f/A 
Value of 
E 
from the 
formula, 
PW 
a/PS 
Value of 
S 
from the 
formula, 
rw. 
4 ad 3 
in 
m lb3 ‘ | inches. 
242 
1005 
500 
1.1 
1122 
4. 5 
243 
1000 
500 
.90 
1220 
4. 6 
244 
Bath-, 1826. 
1000 
540 
.975 
1210 
4.65 
336 
1005 
500 
1.175 
1138 
4. 0 
337 
947 
500 
1.2 
1102 
4 a 2 
338 
1005 
500 
1.125 
1090 
3. 2 
Mean results 
993 
500 
1.079 
1147 
4. 2 
518 
8326459 
2366 
SOONDREE. 
74 
*The two last in- 
1000 
500 
.9 
1250 
5. 5 
75 
ferior specimens, 
991 
500 
1.325 
800 
3. 2 
76 
received at Cossi- 
990 
500 
1.3 
800 
3. 2 
pore Gun-carriage 
agency 1825. 
Mean results 
997 
500 
1 075 
950 
4. 0 
544 
8022336 
1960 
TEAK. 
77 
Pegue ; seasoned, 
750 
450 
1.6 
800 
3. 2 
78 
received at Cossi- 
742 
500 
1.05 
1128 
3. 2 
79 
pore from 1825. 
700 
300 
1.15 
700 
3. 5 
Mean results 
730 
450 
1.266 
876 
3. 3 
660 
6386907 
1806 
80 
From Malabar; sea- 
718 
500 
1.025 
1100 
3. 8 
81 
soned, received at 
720 
500 
1.05 
1 162 
3. 5 
88 
Cossipore in 1825. 
730 
500 
1.275 
1150 
3. 0 
Mean results 
721 
500 
1.116 
1137 
3. 4 
640 
8050403 
2345 
89 
Buzzar; seasoned 
683 
450 
1.125 
1050 
3. 0 
102 
1826. 
688 
500 
1.525 
1150 
3. 8 
ID5 
688 
500 
1.375 
1100 
4. 3 
Mean results 
688 
400 
1.341 
1100 
3. 7 
588 
6471875 
2175 
teak. 
284 
FromMalabar; sea- 
792 
500 
1.075 
1120 
3. 6 
285 
soned 1826. 
747 
500 
1.05 
1036 
2. 6 
286 
792 
500 
1.1 
850 
2. 3 
__ 
Mean results 
743 
500 
1.075 
1002 
2.83 
769 
8357011 
2066 
344 
teak. 
Mug Gun-carriage 
750 
500 
1.0 
1036 
4. 5 
plank; unseasoned, 
736 
500 
1.0 
950 
2. 2 
1827. 
Mean results 
743 
500 
1.05 
993 
3.35 
650 
8556428 
2048 
See the results with Goruckpore Saul at the end of this Table- 
